Advances in Materials Physics and Chemistry, 2012, 2, 35-37 doi:10.4236/ampc.2012.24B010 Published Online December 2012 (http://www.SciRP.org/journal/ampc)
A Sewage Sludge Derived Composite Material for Adsorption of Antibiotics – Kinetics Pengfei Zhang1, Rui Ding1, Mykola Seredych2, Teresa J. Bandosz2 Department of Earth and Atmospheric Sciences, City College of New York, New York, USA 2 Department of Chemistry, City College of New York, New York, USA Email: [email protected]
, [email protected]
ABSTRACT A novel sewage-sludge derived composite material was developed for the adsorptive removal of organic pollutants from water. In this study a batch adsorption study was carried out to examine the kinetics of antibiotics adsorption by this composite material. A pseudo-second order kinetics model fits the data extremely well, suggesting that chemical adsorption, rather than physical adsorption, is likely the main mechanism of the separation process. Keywords: Sewage Sludge; Composite Material; Adsorption Kinetics; Antibiotics; Wastewater Treatment
1. Introduction An estimated 100,000 to 200,000 tons of antibiotics are produced each year  as human and veterinary medicine [2,3], and as much as 30% to 90% of administered antibiotics can be excreted without being metabolized . The excreted antibiotics are often discharged into surface waters or leached into soils and groundwater from manure-based fertilizers or sewage sludge [2, 5], contaminating aquatic and terrestrial environments. Even low concentration of antibiotics in the environment may lead to the development and spreading of antibiotic resistance. Therefore, there is an urgent need to develop advanced treatment technologies that can effectively remove antibiotics and other related pollutants from contaminated water, especially from drinking water sources. In a recent study , we demonstrated that composite materials derived from the pyrolysis of sewage sludge and waste oil sludge were able to simultaneously remove a dozen or so antibiotics from water. The adsorption capacities of these composite materials are comparable to typical granular activated carbons [6,7]. Physical adsorption, reactive adsorption and specific polar interactions were indicated as the mechanisms of the separation process . The objective of this study was to examine the kinetics of antibiotics adsorption by one of those sewage sludge derived composite materials.
2. Materials and Methods 2.1. Composite Material The composite material (SSWO950) was obtained by pyrolysis of a mixture (50:50 ratio based on the wet mass) industrial waste oil sludge (WO) from Newport News Shipyard (Newport News, VA, USA) and dewatered sewage sludge (SS) from Wards Island Water Pollution Control Plant (New York, NY, USA), at 950 oC in a nitrogen atmosphere in a fixed bed (hori*
2.2. Batch Adsorption Experiment Adsorption of a mixture of 11 antibiotics plus 2 anticonvulsants (see Table 1 for the list of compounds) was measured in closed batch systems at room temperature. One mL of the mixture solution (100 mg·L-1 of each compound) was mixed with 0.050 g of the SSWO950 material in amber glass vials. The sample vials were sealed and then shaken on an orbital shaker. Duplicate samples were taken at 2, 4, 6, 8, and 23.5 hours and analyzed for the kinetics study.
2.3. Sample Analysis All samples were analyzed using liquid chromatography-tandem mass spectrometry (LC/MS/MS) with electron spray ionization (ESI) and multiple reaction monitoring (MRM). Details of the analysis can be found in Ding et al. . Table 1. Antibiotics and anticonvulsants tested in this study. Category
Partially supported by the US Environmental Protection Agency.
Copyright © 2012 SciRes.
P. F. ZHANG
2.4. Kinetic Modeling
Table 2. Fitted parameter values from the Pseudo-second order kinetics model.
Both the pseudo-first order and pseudo-second order kinetics models were used to fit the experimental data. The equation for the pseudo-first order model is as follows :
dqt dt k1 qe qt
where qe and qt are the sorption capacities (mg·g-1) at equilibrium and at time t, respectively, and k1 is the rate constant of the pseudo-first order sorption (L·hr-1). Integrating (1) from t = 0 to t and qt = 0 to qt yields: log qe qt log qe k1t
If pseudo-first order kinetics is applicable, then a plot of log(qe-qt) vs. t should yield a straight line and the slope corresponds to k1. Here the sorption capacities determined at 48 hours were used as qe. The equation for the pseudo-second order model is written as follows : dqt dt k2 qe qt
where k2 is the rate constant of the pseudo-second order sorption (g·mg-1·hr-1). Integrating (3) from t = 0 to t and qt = 0 to qt yields: 1 qe qt 1 qe k2t (4)
Rearranging (4) gives the linearized form: t qt 1 k2 qe2 t qe
If pseudo-second order kinetics is applicable, a plot of t/qt vs. t should give a straight line, from which qe and k2 and can be determined from the slope and intercept of the line.
3. Results and Discussion The pseudo-first order kinetics model did not fit the data well (plots not shown), whereas the pseudo-second order kinetics model yielded excellent fits for all compounds (Figure 1, r2 > 0.996), suggesting a chemical adsorption process rather than a physical adsorption process. The fitted qe and k2 values are listed in Table 2. Chlortetracycline, carbamazepine, oxytetracycline, and enrofloxacin appear to have the highest pseudo-second order rate constants
(>45 g·mg-1·hr-1), whereas penicillin-G, primidone, and sulfamethoxazole seem to have the lowest rate constants (